- freely available
Forests 2013, 4(3), 575-594; doi:10.3390/f4030575
Published: 10 July 2013
Abstract: There is a growing interest to use acoustic sensors for selection in tree breeding to ensure high wood quality of future plantations. In this study, we assessed acoustic velocity as a selection trait for the improvement of mechanical wood properties in two 15- and 32-year-old white spruce (Picea glauca [Moench.] Voss) genetic tests. Individual heritability of acoustic velocity was moderate and of the same magnitude as heritability of wood density. Considerable genetic gain could be expected for acoustic velocity and a measure combining velocity and wood density. The relationship between acoustic velocity and cellulose microfibril angle (MFA) was strong on the genetic level and selection based on velocity could effectively improve MFA, which is one of the most important determinants of wood mechanical properties. Although low, the positive relationship between acoustic velocity and tree height presents an interesting opportunity for the improvement of both tree growth and wood quality. On the phenotypic level, MFA was more strongly correlated to acoustic velocity in mature trees than in young trees. The addition of easily obtainable traits such as diameter at breast height (DBH), height-to-diameter ratio as well as wood density to velocity determinations could improve models of MFA at the young and the mature age. We conclude that juvenile acoustic velocity is an appropriate trait to select for wood quality in a tree breeding context.
White spruce (Picea glauca [Moench] Voss) spans the North American continent from Newfoundland to Alaska and is one of the most important boreal conifer species for the Canadian forest industry. White spruce wood is highly valued for pulp and especially for lumber due to its good machining and structural properties . In common with other boreal species, white spruce is very slow growing compared to more temperate species such as radiata pine (Pinus radiata D. Don), loblolly pine (Pinus taeda L.) or even Douglas-fir (Pseudotsuga menziesii [Mirb.] Franco). Tree breeding programs have been established for white spruce since the 1960s in different parts of Canada and the United States, but these have mainly focused on the improvement of growth and adaptive traits, even though faster growth is generally negatively correlated with important wood quality traits such as density and mechanical properties [2,3]. There is therefore a need to include wood traits in tree selection programs to ensure future wood supplies have the appropriate mechanical properties for structural applications and other end uses.
Previous studies have examined the genetic parameters of wood density and its components in white spruce from eastern  and western Canada , where abundant hybridization occurs between white spruce and Engleman spruce (Picea engelmannii Parry ex Engelm.). In more recent work, genetic variation of other wood traits, such as decay resistance , fibre length  or veneer quality  has been studied, although genetic control of those traits was found to be rather low. Moderate to high genetic control of wood traits related to mechanical end uses, such as density and microfibril angle (MFA) [3,8] (in hybrid spruce), or modulus of elasticity (MOE)  (in eastern white spruce) has also been reported. These studies concluded that breeding for certain traits should result in considerable genetic gain and improvement of the next generation’s wood quality.
In advanced breeding generations, selection criteria are constantly adapted in order to improve additional wood quality traits. However, there are two major problems that hinder the application of cost-effective breeding strategies for the improvement of wood quality (Figure 1). The first is the high cost of traditional wood trait evaluation methods, and the second is the length of time before mature wood can be evaluated, especially in slow growing boreal conifers. Since manufacturing investment cycles are far shorter than harvest rotation periods in such species, the development of non-destructive methods for evaluating young trees in order to select for adult wood quality is becoming increasingly important.
1.1. Indirect Assessment Methods
In recent decades, many indirect and non-destructive methods for wood quality evaluation on standing trees have been developed and most were reviewed by Wessels et al. . Many of these techniques have also been evaluated for tree breeding. For example, spectroscopic analysis for the prediction of wood chemical composition (e.g., ), or the assessment of mechanical wood traits (e.g., [12,13]) using increment cores. Such approaches, however, require the development of models and then further validation, which can be complicated and expensive depending on the trait of interest and its variation in the breeding populations. Other in-field assessment methods such as Pilodyn pin penetration or drill resistance measurements have also been used in genetic studies, since both are strongly correlated to wood density (e.g., [14,15]).
Other promising methods for the evaluation of wood mechanical properties are tools that can measure the transit time of sound waves in lumber or standing trees. These tools are easier to handle than traditional destructive mechanical testing. Acoustic velocity is directly related to dynamic wood stiffness, or modulus of elasticity (MOE) , which is highly correlated with modulus of rupture (MOR). Since MOE and MOR are affected by intrinsic clear-wood properties such as microfibril angle and wood density, the latter are very important determinants of timber performance for structural end-uses . Both MOE and MOR have been noted to increase linearly with wood density . Alteyrac et al. , for example, reported that MFA explained 50% and more than 70% of variation in black spruce MOR and MOE, respectively. However, the mechanical properties of lumber pieces may be reduced by the occurrence of knots, depending on their size and location [17,18]. In contrast, knots have very little influence on acoustic velocity because the dilatational wave tends to take the fastest path of travel around local defects. In consequence, an acoustic velocity measurement gives a mean estimate of MOE over the entire stem section in which it has been measured, but it may overestimate local minima due to knots or other defects in pieces of solid wood .
Numerous studies have investigated the links between acoustic measurements in standing trees, logs and the mechanical properties of wood samples from the same stem. A strong relationship between acoustic measurements on standing trees and felled logs was reported by Grabianowski et al.  in radiata pine. Using acoustic velocity in logs, Achim et al.  reported a strong correlation between dynamic and static MOE in trembling aspen (Populus tremuloides Michx.), and good correlations were reported between standing tree acoustic velocity and MOR in Scots pine (Pinus sylvestris L.) .
Largely due to these encouraging results, the use of acoustic measurements for the evaluation of mechanical wood properties has promising applications in a tree breeding context [24,25,26]. Already, acoustic devices are being deployed on an operational basis in various tree improvement programs, particularly for fast growing pine species, such as radiata pine . However, somewhat contrasting estimates of genetic parameters, such as heritability, have been reported for different species. For example, heritability values for acoustic velocity ranged from below 0.2 in Douglas-fir  to almost 0.6 in radiata pine . To our knowledge, no genetic study has directly assessed the use of acoustics in white spruce breeding programs.
1.2. Early Selection
Besides the cost-effective evaluation of traits, early selection efficiency i.e., the possibility to select individuals at a juvenile age that will have superior rotation-age properties plays an important role in tree breeding. Most wood traits in conifers vary systematically from juvenility to maturity . These patterns are essentially dependent on cambial age but may also be influenced by environmental variables and other traits, such as annual ring-width [31,32]. In order to evaluate if adult traits are linked to juvenile traits and whether these relationships can be used as a basis for early selection, a common practice in genetics is to analyze age–age correlations. In white spruce, mechanical wood traits, such as MOE and MOR, along with microstructural properties, such as MFA, show high age–age correlation and thus have strong potential for effective early selection . For such purposes, non-destructive techniques such as the acoustic evaluation of standing trees to indirectly measure stiffness carry a clear advantage over destructive methods. Indeed, Li et al.  found velocity instruments to be excellent tools for the evaluation of wood stiffness in 8-year-old slash pine. Similar results were reported by Eckard et al.  in a study on 8-year-old loblolly pine clones.
At the start of the current study, it was not known how a combination of slow growth, small diameter stems and a high incidence of live branches along the whole length of the stem would influence the accuracy of the velocity measurements and, consequently, the suitability of acoustic tools for use in breeding programmes for slow-growing boreal conifers. The overall objective of this study was to assess whether early selection based on acoustic velocity can improve white spruce mechanical wood properties. Specific objectives were (1) to evaluate the selection efficiency of acoustic tools in young trees of this species, and (2) investigate the relationship between acoustic velocity, tree growth-related variables and mechanical wood traits in young and mature white spruce trees.
2. Materials and Methods
Young and mature white spruce trees from three sites in the province of Quebec, Canada, were used in the analyses. The sites were part of two different progeny trials. Young trees were sampled from two sites belonging to a full-sib trial planted in 1999, so trees were 15 years old at the time of sampling. One of these sites was located near Saint-Casimir, Quebec, in the maple-basswood ecological zone, and the other was close to Cabano, Quebec, in the balsam fir-yellow birch zone. The trials were laid out as randomized complete block designs, where each family was represented by five trees in one row-plot per block. Spacing between trees was 2 m in all directions. In order to avoid unbalanced data due to mortality and missing families, we concentrated our sampling on 5 blocks at Saint-Casimir and 6 blocks at Cabano. In total, between 14 and 16 trees per site were sampled from each of the 59 full-sib families, giving a total sample of 1534 young trees.
Data from mature trees were obtained from a site near Mirabel, Quebec, in the maple—bitternut hickory—dominated ecological zone. This site is part of a series of half-sib provenance progeny trials established in the early 1980s, hence trees were 32 years old at the time of sampling. The trial was laid out as a randomized complete block design in which each family was initially represented by a row-plot with four trees in each block. Spacing within plots was 1.5 m and 2.5 m between row-plots. In 2005, around 50% of trees in each family were removed in a thinning intervention and the remaining trees were pruned up to 2 m. In total, 102 mature trees were sampled from 40 half-sib families (representing 2 to 3 trees per family).
At all three sites, diameter at breast height (DBH, measured 1.3 m from ground level), total tree height and acoustic velocity were recorded for all sample trees. In addition, increment cores were taken at 1.3 m from each of the young trees and mature trees for X-ray diffraction and densitometry measurements.
2.2. Measurement of Standing Tree Acoustic Velocity
The Hitman ST300 tool (Fibregen, Christchurch, New Zealand) was used to obtain acoustic velocity measurements on the north face of each stem. In order to allow for perfect alignment and accurate distance measurements between the two probes of the device, some living branches had to be removed prior to testing of the young trees. The probes were inserted approximately 4 cm into the stem and aligned vertically around breast height at a distance of approximately 50 to 60 cm apart. Accelerometers attached to the probes record the transit time of an acoustic wave induced by a hammer blow. For each tree, 24 readings were taken on the north face of each stem and the average of these was used. Measurements were taken on each experimental site during a two-week period in June/July 2012, thus avoiding severe temperature differences that might have affected velocity measurements .
The dynamic modulus of elasticity is related to acoustic velocity and density by the one-dimensional wave equation:
2.3. Determination of Wood Density Using Scanning X-Ray Densitometry
Density was measured on samples from young and mature trees using two separate scanning X-ray densitometry systems. Increment cores were cut to a thickness of either 1.68 mm (young trees) or 2 mm (mature trees) in the tangential direction with a twin blade pneumatic saw. They were then Soxhlet extracted overnight with acetone, and conditioned to approximately 7% moisture content before scanning. The samples from the young trees were scanned from pith to bark along the radial face at a resolution of 25 µm in a QTRS-01X Tree Ring Analyzer (Quintek Measurement Systems Inc., Knoxville, TN, USA). The mature tree samples were air-dried (20 °C and 40% relative humidity, which corresponds to an approximate equilibrium moisture content of 8%) and scanned at a resolution of 25 µm using the SilviScan-3TM system [36,37] located at the FPInnovations laboratory in Vancouver, British Columbia. This system combines image analysis, X-ray densitometry and X-ray diffractometry to obtain pith-to-bark profiles for wood density, microfibril angle (MFA) and Silviscan modulus of elasticity (MOESS). From the density profiles, the limits of the annual growth rings were determined together with the relative proportions of earlywood and latewood in each annual ring using in-house data processing routines. The transition from earlywood to latewood was thereby found as the mean of the minimum and the maximum density in a growth ring.
2.4. Determination of Microfibril Angle Using X-Ray Diffraction
For the mature trees, samples were scanned from pith to bark using the SilviScan-3 X-ray diffractometer, and the mean MFA was calculated over 3-mm intervals. The diffraction profiles provide information about the orientation of the cellulose microfibrils in the S2 layer of the secondary cell wall . The MFA in samples from young trees was measured by scanning the radial face of the last complete growth ring closest to the bark with a D8 Discover X-ray diffractometer (Bruker AXS, Madison, WI, USA) . Diffraction profiles for a few samples were first calibrated by comparison with values obtained using compound light microscopy, before the complete population of samples was scanned.
2.5. Quantitative Genetic Analyses
Variance and covariance components for genetic analyses of this manuscript were estimated with the SAS MIXED procedure . Data from young trees were analyzed in a combined site analysis following the model:
Individual heritability (h²individual) was estimated according to the equation:
2.6. Phenotypic Analyses and Modeling
In order to assess the value of acoustic velocity for description of white spruce wood quality, linear mixed-effects models were separately fitted to the data from young and old trees to determine the relationship between MFA and acoustic velocity and between MOESS and acoustic velocity. Using matrix notation, such models can be expressed generally as :
In the models, the effect of tree size was assessed by the inclusion both DBH and tree height/diameter ratio (HD) as explanatory variables. Area-weighted core mean density was also screened as a covariate. Model selection was based on Akaike’s Information Criterion (AIC)  and fit indices (R2) calculated from the fixed, and from the fixed plus random effects of the models .
Table 1 gives an overview of wood trait means and coefficients of variation (CV) at the three sites analyzed in this study. As expected, acoustic velocity was higher, and MFA lower, in the mature trees. Earlywood density showed similar dispersion across all three sites. Average ring density as well as latewood density and latewood width were higher in the mature trees. The CVs were generally higher in young trees for all traits expect for earlywood density and MFA. Of the young trees, those from the Cabano plantation were established in a more heterogeneous environment, which was reflected in slower height and diameter growth, lower acoustic velocity, higher MFA and slightly higher overall variation compared to the trees from Saint-Casimir.
|Table 1. Means and coefficient of variation (CV, in parentheses) of wood traits at each site.|
|Mature trees||Young trees|
|Ring Number||22.09 (6.75)||7.40 (11.18)||7.59 (11.74)|
|Velocity [km s−1]||4.17 (10.34)||2.70 (13.69)||2.87 (12.24)|
|MFA [°]||19.51 (21.94)||36.25 (9.24)||33.09 (8.53)|
|MOESS [GPa]||8.80 (20.97)||–||–|
|Vel² × Dens [GPa]||7.30 (23.47)||2.84 (28.29)||3.33 (27.03)|
|Density [kg m−³]||413.91 (7.49)||386.90 (9.73)||396.13 (7.31)|
|EW density [kg m−³]||361.19 (7.01)||361.77 (7.32)||368.84 (6.24)|
|LW density [kg m−³]||713.55 (6.59)||661.11 (3.74)||691.64 (3.7)|
|Ring width [mm]||3.74 (16.46)||4.3 (20.03)||4.21 (19.72)|
|EW width [mm]||3.27 (17.66)||3.87 (23.77)||3.82 (21.31)|
|LW width [mm]||0.62 (24.3)||0.43 (48.5)||0.39 (34.5)|
|EW percentage||0.83 (4.03)||0.89 (7.16)||0.90 (4.04)|
|DBH [cm]||18.89 (15.89)||7.48 (21.79)||7.58 (22.24)|
|Height [m]||12.62 (12.64)||4.91 (16.09)||5.64 (17.58)|
MFA: microfibril angle; MOESS: SilviScan modulus of elasticity; EW: earlywood; LW: latewood; DBH: tree diameter at breast height. Density is the mean wood density combining, the density of earlywood and latewood.
3.1. Genetic Parameters for Young Trees
Parameter estimates were obtained from trees of 59 controlled pollinated crosses that are currently being evaluated in the Quebec white spruce breeding program. Table 2 presents individual heritability estimates as well as genetic and phenotypic correlations for the individual tree level. Table 3 contains family heritability and estimates for genetic gain based on family means. Associated errors of the estimates were rather low and varied between 0 and 0.19 (Table 2, Table 3). Moderate individual heritability estimates were found for tree height and for most wood traits (Table 2); the highest heritability estimates were for acoustic velocity (h² = 0.38) and earlywood density (h² = 0.41). The heritability of MFA (h² = 0.22) was rather low and of the same range as that of growth increment-related traits, such as DBH, average ring width and earlywood width. Latewood density and width were also under weak genetic control.
Acoustic velocity gave moderate phenotypic correlation (rP = −0.49) and strong genetic correlation (rG = −0.84) with MFA (Table 2) indicating that both traits may be controlled by largely the same set of genes. However, the relationship between velocity and wood density as well as other growth-related traits was rather weak. While the correlation between velocity and radial increment (ring width and DBH) was very low in young trees, results indicate a positive but weak correlation between height growth and acoustic velocity (rP = 0.12, rG = 0.17). At the genetic level, faster growth was associated with low MFA, indicating a tendency for higher mechanical properties in faster-growing genotypes. Moderate negative correlations were found for MFA with DBH (rG = −0.38), height (rG = −0.44), and ring width (rG = −0.37), as well as with earlywood width (rG = −0.34) and earlywood percentage (rG = −0.57); however, the equivalent phenotypic correlations were quite weak.
|Table 2. Genetic parameter estimates for the combined site analyses of young trees. Genetic correlations are above and phenotypic correlations are below the diagonal. Individual heritability estimates are in bold on the diagonal. Errors associated to correlations and heritability estimates are in parentheses.|
|Velocity||MFA||Vel² × Dens||Density||EW density||LW density||Ring width||EW width||LW width||EW percentage||DBH||Height|
|Velocity||0.38 (0.07)||−0.84 (0.07)||0.96 (0.01)||0.13 (0.03)||0.20 (0.02)||0.10 (0.18)||0.03 (0.17)||0.06 (0.17)||−0.18 (0.17)||0.19 (0.18)||0.01 (0.02)||0.17 (0.02)|
|MFA||−0.49 (0.02)||0.22 (0.05)||−0.72 (0.09)||0.23 (0.16)||0.13 (0.16)||0.05 (0.19)||−0.37 (0.16)||−0.44 (0.16)||0.38 (0.16)||−0.57 (0.15)||−0.38 (0.16)||−0.44 (0.05)|
|Vel² × Dens||0.95 (0.00)||−0.45 (0.03)||0.36 (0.07)||0.38 (0.14)||0.44 (0.13)||0.19 (0.17)||−0.09 (0.17)||−0.10 (0.17)||0.02 (0.17)||−0.10 (0.02)||−0.06 (0.17)||0.16 (0.16)|
|Density||0.12 (0.01)||0.04 (0.03)||0.41 (0.03)||0.32 (0.06)||0.99 (0.01)||0.36 (0.16)||−0.39 (0.14)||−0.51 (0.13)||0.70 (0.10)||−0.86 (0.06)||−0.41 (0.14)||−0.28 (0.15)|
|EW Density||0.14 (0.01)||0.04 (0.03)||0.40 (0.03)||0.94 (0.01)||0.41 (0.07)||0.31 (0.16)||−0.36 (0.05)||−0.48 (0.13)||0.63 (0.11)||−0.78 (0.08)||−0.40 (0.14)||−0.28 (0.15)|
|LW Density||0.22 (0.03)||−0.17 (0.03)||0.30 (0.03)||0.35 (0.03)||0.22 (0.03)||0.14 (0.04)||−0.14 (0.19)||−0.21 (0.19)||0.40 (0.17)||−0.38 (0.18)||−0.04 (0.19)||0.10 (0.18)|
|Ring width||−0.11 (0.03)||−0.09 (0.03)||−0.23 (0.03)||−0.50 (0.02)||−0.45 (0.02)||−0.20 (0.03)||0.23 (0.05)||0.99 (0.01)||0.15 (0.18)||0.42 (0.16)||0.96 (0.01)||0.83 (0.06)|
|EW width||−0.10 (0.03)||−0.10 (0.03)||−0.26 (0.03)||−0.60 (0.02)||−0.54 (0.02)||−0.23 (0.03)||0.98 (0.00)||0.22 (0.05)||−0.01 (0.19)||0.56 (0.13)||0.95 (0.03)||0.79 (0.03)|
|LW width||−0.01 (0.03)||0.07 (0.03)||0.17 (0.03)||0.63 (0.02)||0.50 (0.02)||0.19 (0.03)||−0.04 (0.03)||−0.22 (0.03)||0.16 (0.04)||−0.83 (0.06)||0.15 (0.18)||0.19 (0.17)|
|EW percentage||−0.01 (0.03)||−0.10 (0.03)||−0.21 (0.03)||−0.78 (0.01)||−0.62 (0.02)||−0.25 (0.03)||0.46 (0.02)||0.62 (0.02)||−0.87 (0.01)||0.12 (0.04)||0.42 (0.16)||0.28 (0.03)|
|DBH||−0.05 (0.00)||−0.12 (0.03)||−0.15 (0.03)||−0.40 (0.03)||−0.40 (0.03)||−0.06 (0.03)||0.80 (0.01)||0.78 (0.01)||−0.01 (0.03)||0.35 (0.02)||0.23 (0.05)||0.93 (0.03)|
|Height||0.12 (0.01)||−0.19 (0.01)||0.06 (0.04)||−0.31 (0.03)||−0.31 (0.03)||0.02 (0.03)||0.66 (0.02)||0.63 (0.03)||0.04 (0.03)||0.27 (0.02)||0.82 (0.01)||0.33 (0.07)|
Similarly, there was a weak to moderate genetic link between MFA and density (rG = 0.23) and between MFA and latewood width (rG = 0.38). Their phenotypic correlations were again close to zero. Genetic parameters of Vel² × Dens were close to the estimates for its individual components, especially velocity. However, it is interesting to note that while phenotypic correlations between Vel² × Dens and radial growth parameters (i.e., ring width, earlywood percentage and DBH) were weak and negative, virtually no correlation was found on the genetic level.
Genetic and phenotypic correlations were strongly positive between density and latewood width (rP = 0.35, rG = 0.70) and moderately negative for density and traits related to growth, which was expected. Additionally, earlywood and latewood width often showed opposite correlations with the same traits especially on the genetic level.
|Table 3. Estimates of family heritability and genetic gain based on family means in young trees. A selection intensity of α = 0.05 was used for the calculation of gain.|
|Vel² × Dens||0.77 (0.04)||20.17|
|EW density||0.82 (0.04)||5.44|
|LW density||0.60 (0.08)||1.44|
|Ring width||0.66 (0.06)||10.71|
|EW width||0.64 (0.06)||10.46|
|LW width||0.67 (0.06)||18.64|
|EW percentage||0.58 (0.08)||2.04|
Based on the heritability estimates and the phenotypic variance components of wood traits, we assessed the expected genetic gain under a standardized selection scenario (i = 2.06 in Equation 6, which means that about 5% of individuals (Table 4) or families (Table 3) are retained during selection. Despite the moderate individual heritability estimates of most traits analyzed in this study, the expected genetic gain for a specific trait over its mean value varied from about 1% to almost 20% (for selection on the individual tree level and the family level). For MFA, the expected gain was almost 5%, while a gain of more than 10% could be expected when selection is based on growth-related traits. The expected gain for density was approximately 5.5%. Selection for acoustic velocity could improve this trait by almost 10%, which is encouraging for its practical application in a tree breeding program. The highest gain was expected for Vel² × Dens, which could be improved by 20% in this selection scenario (Table 4).
Heritability estimates based on family means were moderate to high for all traits (Table 3) and more than twice as big as their individual counterparts. The relative differences in genetic control between traits did not change. The estimated genetic gain was of the same magnitude as the genetic response expected on the individual tree level. According to our results, a higher gain could be expected based on selection of entire families for DBH (GInd = 10.20%, GFam = 12.15%) and for MFA (GInd = 4.02%, GFam = 4.96%).
Table 4 also shows the selection efficiency of different traits that could be obtained by indirect selection of another trait. Selection based on acoustic velocity had a small effect on both ring width and DBH, and only 14% of the total possible gain in wood density was predicted when selection was based on velocity alone. At the same time, 18% of the possible gain in tree height was estimated. However, the use of acoustic velocity had rather little effect on other growth- and density-related traits. In contrast, the indirect selection efficiency for MFA was theoretically greater than 100%, indicating that genetic gains for MFA were higher through the indirect selection for acoustic velocity than through direct selection for MFA itself. This was related to the important difference in genetic control of both MFA and velocity. Selecting for lower MFA values at the same time indirectly improved the gain from DBH and height by about a third in each case (Eind = −0.37 and Eind = −0.35, respectively). A selection strategy for improving tree height or DBH could at the same time produce gains of earlywood ring width (respectively Eind = 0.96, Eind = 1.00) and overall ring width (respectively Eind = 0.98, Eind = 0.99). This strategy also resulted in a loss in wood density which could counterbalance a third of its possible gain and had a small impact on velocity (height selection Eind = 0.16, DBH, Eind = 0.00).
|Table 4. Efficiency of indirect selection among different wood traits. Estimates for genetic gain (in percent of the population mean) are in bold on the diagonal.|
|Indirect effect on:||Density||EW density||LW density||Ring width||EW width||LW width||EW percentage||DBH||Height|
|Velocity||MFA||Vel² × Dens|
|Vel² × Dens||0.93||−0.92||19.98||0.40||0.42||0.31||−0.11||−0.12||0.03||−0.17||−0.07||0.17|
3.2. Phenotypic Modeling of Mechanical Wood Traits
In the previous section, genetic and phenotypic correlations between acoustic velocity and MFA have been shown to differ in magnitude. To better understand why phenotypic correlations between both traits were considerably weaker than their genotypic counterpart, we investigated which traits—besides velocity—may influence mechanical wood quality on the observational level.
3.2.1. Models for Predicting MFA in Young Trees
There was a weak to moderate relationship between acoustic velocity and MFA in young trees (Table 5). The best model for predicting MFA from velocity (model 4) contained both velocity and HD-ratio in the fixed effects, which was slightly better in terms of AIC and fit indices than the model with velocity and DBH as predictors (model 3). The average density of the last rings was not a significant predictor (model 5). Overall, the amount of variation explained by the fixed effects was between 24.1 and 25.3%, with only a small increase if fit indices included the family random effect (Table 3).
|Table 5. Models for predicting MFA in young trees showing parameter estimates, AIC and fit indices calculated from the fixed, and fixed plus random effects.|
|Model||Fixed effects parameters||AIC||Fit indices ( R²)|
|1||47.16 **||−4.52 **||–||–||–||–||8388.83||0.241||0.276|
|2||40.86 **||–||−0.80 **||–||–||–||8389.99||0.240||0.276|
|3||48.39 **||−4.53 **||–||−0.02 *||–||–||8381.12||0.246||0.279|
|4||49.34 **||−4.13 **||–||–||−0.46 **||–||8359.31||0.253||0.293|
|5||48.05 **||−4.50 **||–||–||–||−0.002 ns||8389.76||0.240||0.278|
** P-value < 0.001; * P-value < 0.01; ns P-value > 0.1.
3.2.2. Models for Predicting MFA and MOESS in Mature Trees
The relationship between MFA and acoustic velocity was moderate to strong in mature trees (Table 6). Fit indices of fixed effects ranged from 52.5% to 54.6%, considerably higher than in the models for juvenile trees. Similar to juvenile trees, the HD-ratio was significant in the mature trees; however, the best model contained acoustic velocity as the only independent variable. The models describing MOE were slightly better than the MFA models and their fit indices of fixed effects varied between 55.2% and 62.5%. Besides acoustic velocity, DBH was found to significantly contribute to explaining MOE. The best model included the HD-ratio and the fixed effects explained more than 62% of the variation of MOE. Including the family random effect increased the fit indices by around 10% for MFA models or by 15% for MOE models. In any case, using the square of acoustic velocity for modelling MFA or MOE did not significantly improve the model fit in either the young or the mature trees.
|Table 6. Models for predicting area-weighted core mean microfibril angle (MFA) and modulus of elasticity (MOE) in mature trees showing parameter estimates, AIC and fit indices calculated from the fixed, and fixed plus random effects.|
|Trait||Model||Fixed effects parameters||AIC||Fit indices ( R²)|
|MFA||1||48.55 **||−6.74 **||–||–||–||–||512.81||0.538||0.647|
|2||34.23 **||–||−0.78 **||–||–||–||515.64||0.525||0.635|
|3||46.23 **||−6.68 **||–||0.11 ns||–||–||513.51||0.546||0.635|
|4||49.56 **||−6.52 **||–||–||−2.84 **||–||514.16||0.543||0.632|
|5||45.78 **||−6.88 **||–||–||–||−0.008 ns||514.13||0.539||0.660|
|MOE||6||−3.76 **||2.92 **||–||–||–||–||328.72||0.558||0.771|
|7||2.40 **||–||0.34 **||–||–||–||330.57||0.552||0.762|
|8||−1.19 ns||2.86 **||–||−0.12 *||–||–||320.88||0.615||0.759|
|9||−5.41 **||2.55 **||–||–||4.78 **||–||318.79||0.625||0.760|
** P-value < 0.001; * P-value < 0.01; ns P-value > 0.1.
Genetic parameter estimates and phenotypic prediction models from 15-year-old and 32-year-old white spruce progeny tests were used to evaluate acoustic velocity as a selection trait for wood quality. The moderate heritability of acoustic velocity, the promising genetic gains and the strong relationship with MFA and MOE make it possible to use it as a surrogate for mechanical properties in white spruce tree improvement strategies. Heritability of acoustic velocity in young white spruce (h² = 0.38) was found to be of the same magnitude as estimates for other wood traits . A comparable degree of genetic control of acoustic velocity was reported by Li et al.  from a study in young slash pine (h² = 0.42), although somewhat higher heritability was estimated in young radiata pine (h² = 0.47) by Kumar et al. .
The moderate genetic control of velocity led to an expected gain that was of the same magnitude as the expected improvement of the growth traits DBH and height. Combining acoustic velocity and density to an approximate measure of dynamic MOE (Vel² × Dens) increased the variation that is accessible for selection and led to the highest expected gain in the panel of analyzed traits. However, the use of density as an early selection trait requires caution, since its selection efficiency at a very early age has been found to be low in a previous work on white spruce . The rather small correlation between acoustic velocity and wood density in this study is in contrast to earlier results on Douglas-fir . This is probably linked to differences in wood structure, since white spruce has lower density, a more gradual earlywood–latewood transition and a lower latewood percentage than Douglas-fir. In addition, wood density in spruce species typically follows the “Type II” pattern of a rapid decline from a maximum value near the pith followed by a gradual increase to an intermediate value . The high density wood close to the pith also has the characteristically high MFA values associated with compression wood . Thus, early selection for density alone could be counterproductive because of the potential to select families that are prone to producing compression wood. The positive relationship between density and MFA on the genetic level casts further doubt on the utility of density for early selection of mechanical properties. Hence, the combined measurement Vel² × Dens may present a way to simultaneously select for high stiffness and high density, to identify individuals with superior mechanical properties but screening out high density, low stiffness individuals.
Direct selection based on MFA presents another possible strategy for wood quality improvement. Low MFA—and therefore higher stiffness—is moderately related to height and DBH, especially on the genotypic level. At first glance, this may appear counterintuitive because faster growth is usually associated with lower strength and stiffness. But in this study on young white spruce, more vigorous genotypes, especially those with a superior height growth, are thought to form less compression wood because they are already better positioned in the competition for light . They probably also started to produce wood with a less juvenile character at breast height compared to slower growing individuals. Overall, MFA has good early selection efficiency . Selection for MFA could therefore be easily combined with growth improvement strategies. Nevertheless, these gains are offset by a comparably small expected genetic gain for MFA on the individual and family mean levels in this dataset. This is most likely due to the rather weak heritability and low variation of this trait, especially in the young trees where only the MFA of the last complete ring was measured.
The relationships between wood density and growth-related traits, such as DBH, height, ring width, as well as earlywood width and its proportion, are similar to earlier reports [2,8]. More vigorous trees tend to allocate their resources into increased radial increment and height growth, and produce wood of lower density .
The negative correlation between growth rate and wood density is problematic in a tree breeding context. Density, being related to the mechanical traits MOE and MOR, has traditionally been used as an easily measurable trait in order to improve wood quality . Different authors have attempted to find ways around this problem, for example by considering individual density components or traits that influence wood density. Nevertheless, Ivkovich et al.  found no particular benefits of using wood anatomy to solve the problem.
Recent advances in clonal forestry mean that multiple copies of individuals or lines that do not follow the general correlation trend can be produced. Park et al.  identified several fast-growing white spruce clones that maintained above-average density. However, clonal methods are relatively costly, so may only be economically profitable for intensely managed plantations and less suitable for mass reforestation on extensively managed sites. Acoustic velocity presents an interesting alternative to wood density measurements as its correlations with diameter increment were weak. At the same time the relationship between height growth and velocity was positive. Although it was weak in this study, a positive trend between tree height and velocity has been already observed in Douglas-fir  and slash pine . Future selection strategies may profit from acoustic velocity determination because it is more closely related to mechanical traits than wood density alone . This is also shown by insignificance of density in the phenotypic prediction models in the juvenile and the mature trees.
The low to moderate phenotypic relationship between acoustic velocity and MFA is in contrast to the results on the genetic level, which indicate that MFA could be successfully improved by selection for velocity. Environmental influences appear to have attenuated the genetic relationship between both traits. The low R2 in the MFA models for young trees is probably also related to the fact that MFA measurements were made on a single growth ring, compared to the large variation in MFA and MOESS in the mature trees. The addition of other easily measurable traits could not considerably ameliorate model fit for juvenile MFA. In MFA models that included both velocity and diameter as predictors, diameter was the only significant variable for juvenile trees. A significant influence of DBH on adult tree MOE has been reported in previous studies on black spruce [49,50]. Slenderness (HD-ratio) was an important predictor for mechanical wood traits in this study. More slender stems tend to be stiffer and thus have lower MFA in order to support the momentum resulting from the crown. Alternatively, this could be related to the properties of the acoustic wave as it propagates within the stem, since, for a given stiffness, acoustic velocity can be mediated by the ratio between tree diameter and the distance between the probes . The significance of the HD-ratio indicates that this variable is complementary to acoustic velocity for description of mechanical wood quality. This also agrees with the low correlation between growth and velocity and further encourages the use of acoustic velocity besides growth traits in tree improvement.
In contrast to what may be expected from the theoretical relationship of acoustic velocity and mechanical wood traits (Equation 1) the square of velocity did not improve MFA and MOE models in this study. But this may be different when more heterogeneous samples from different ages are considered and the variation in both traits is consequently higher. Additionally, the difference in model fit between juvenile trees and adult trees suggest an evolution of the link between MFA and velocity on the phenotypic level with tree age. Age–age correlations should therefore be monitored more closely in future studies.
Earlier reports on the use of acoustic techniques on young trees using the same or similar tools were based on fast growing pine species with larger stem diameters [34,45,51] than diameters of the young trees in this study. We thus needed to evaluate if acoustic velocity could be measured with a sufficient precision in order to make selection for wood quality in more slowly growing trees. We initially expected high degree of variation of acoustic velocity in young white spruce due to the presence of large numbers of branches. Defects or knots may prevent an optimal propagation of the sound wave especially in small diameter stems. Lindström et al.  mentioned that density variations may weaken velocity measurements and hinder the detection of good quality stems. But the results of this study indicate that acoustic velocity is a useful tool for genetic improvement of wood quality also in slow growing boreal species. Velocity measurements were apparently of good precision also in small trees which is in accordance to the results by Zhang et al.  who noted a more uniform propagation of sound in smaller stems of red pine.
The occurrence of compression wood in juvenile stems is often made responsible for weaker genetic parameters in the juvenile wood than in adult wood for example. Apiolaza et al.  separately analyzed compression wood and opposite wood from systematically leaning radiata pine trees. The authors concluded that their approach reduces the noise of random occurrence of compression and opposite wood in juvenile stems. Although this approach may be too costly for many tree improvement programs, it may help to more precisely separate environmental effects and facilitate the identification of superior or inferior trees in future generations. This could possibly improve phenotypic prediction models at the juvenile age. Nevertheless, several strong genetic relationships were presented in this study which indicates a good power of detection of genetic effects in our experimental layout. Additionally, low errors were associated to heritability and correlation estimates. The precision is probably due to the high number of trees per family chosen for this study following the findings by Perron et al. .
Acoustic tools offer a cost-effective way to screen numerous trees in a breeding context and thus to select the individuals with superior wood mechanical traits, such as MFA and dynamic MOE. The results of this study show that acoustic velocity is a reliable trait for indirect early selection of wood quality in slow growing boreal species such as white spruce. Our findings also suggest rethinking the often stated negative correlation between growth and wood quality traits: the weak but positive correlation between acoustic velocity and tree height offers the opportunity to improve both, wood quality and growth and to avoid the contrasting correlation between growth and wood density. As acoustic velocity is more strongly related to the mechanically important MFA and dynamic MOE, it appears to be a good selection trait to provide future plantations with a genetically improved stock and to avoid a decline of wood quality.
Authors thank Marie-Hélène Galibois for help with acoustic measurements and preliminary analysis of the data. We also thank Roger Gagné, André Beaumont and Sébastien Clément for sampling and databasing. Funding was partly obtained from the Fonds québecois de recherche sur la nature et les technologies (AA, JB, JM), from Genome Canada and Génome Québec for the SMarTForests project (JB, JM) and the Canadian Wood Fibre Centre (JB).
Conflict of Interest
The authors declare no conflict of interest.
- Zhang, S.Y.; Koubaa, A. Softwoods of Eastern Canada: Their Silvics, Characteristics, Manufacturing and End-Uses; FPInnovations–Forintek Division: Québec, Canada, 2008.
- Corriveau, A.; Beaulieu, J.; Daoust, G. Heritability and genetic correlations of wood characters of Upper Ottawa Valley white spruce populations grown in Quebec. For. Chron. 1991, 67, 698–705.
- Ivkovich, M.; Namkoong, G.; Koshy, M. Genetic variation in wood properties of interior spruce. II. Tracheid characteristics. Can. J. For. Res. 2002, 32, 2128–2139, doi:10.1139/x02-139.
- Yanchuk, A.D.; Kiss, G.K. Genetic variation in growth and wood specific gravity and its utility in the improvement of interior spruce in British Columbia. Silvae Genet. 1993, 42, 141–148.
- Yu, Q.; Yang, D.Q.; Zhang, S.Y.; Beaulieu, J.; Duchesne, I. Genetic variation in decay resistance and its correlation to wood density and growth in white spruce. Can. J. For. Res. 2003, 33, 2177–2183, doi:10.1139/x03-150.
- Beaulieu, J. Genetic variation in tracheid length and relationships with growth and wood traits in eastern white spruce (Picea glauca). Wood Fib. Sci. 2003, 35, 609–616.
- Zhang, S.Y.; Yu, Q.; Beaulieu, J. Genetic variation in veneer quality and its correlation to growth in white spruce. Can. J. For. Res. 2004, 34, 1311–1318, doi:10.1139/x04-015.
- Ivkovich, M.; Namkoong, G.; Koshy, M. Genetic variation in wood properties of interior spruce. I. Growth, latewood percentage, and wood density. Can. J. For. Res. 2002, 32, 2116–2127, doi:10.1139/x02-138.
- Lenz, P.; Cloutier, A.; MacKay, J.; Beaulieu, J. Genetic control of wood properties in Picea glauca—An analysis of trends with cambial age. Can. J. For. Res. 2010, 40, 703–715, doi:10.1139/X10-014.
- Wessels, C.B.; Malan, F.S.; Rypstra, T. A review of measurement methods used on standing trees for the prediction of some mechanical properties of timber. Eur. J. For. Res. 2011, 130, 881–893, doi:10.1007/s10342-011-0484-6.
- Jones, P.D.; Schimleck, L.R.; Peter, G.F.; Daniels, R.F.; Clark, A. Nondestructive estimation of wood chemical composition of sections of radial wood strips by diffuse reflectance near infrared spectroscopy. Wood Sci. Technol. 2006, 40, 709–720.
- Schimleck, L.R.; Mora, C.; Daniels, R.F. Estimation of the physical wood properties of green Pinus taeda radial samples by near infrared spectroscopy. Can. J. For. Res. 2003, 33, 2297–2305, doi:10.1139/x03-173.
- Poke, F.S.; Potts, B.M.; Vaillancourt, R.E.; Raymond, C.A. Genetic parameters for lignin, extractives and decay in Eucalyptus globulus. Ann. For. Sci. 2006, 63, 813–821, doi:10.1051/forest:2006080.
- Costa E Silva, J.; Borralho, N.M.G.; Wellendorf, H. Genetic parameter estimates for diameter growth, pilodyn penetration and spiral grain in Picea abies (L.) Karst. Silvae Genet. 2000, 49, 29–36.
- Isik, F.; Li, B. Rapid assessment of wood density of live trees using the Resistograph for selection in tree improvement programs. Can. J. For. Res. 2003, 33, 2426–2435, doi:10.1139/x03-176.
- Bucur, V. Acoustics of Wood; Springer-Verlag: Berlin, Germany, 2006.
- Panshin, A.J.; Zeeuw, C. Textbook of Wood Technology; McGraw-Hill Book Co.: New York, NY, USA, 1980; p. 722.
- Bowyer, J.L.; Shmulsky, R.; Haygreen, J.G. Forest Products and Wood Science: An Introduction; Blackwell Publishing: Ames, IO, USA, 2007.
- Alteyrac, J.; Cloutier, A.; Ung, C.H.; Zhang, S.Y. Mechanical properties in relation to selected wood characteristics of black spruce. Wood Fib. Sci. 2006, 38, 229–237.
- Chauhan, S.S.; Walker, J.C.F. Variations in acoustic velocity and density with age, and their interrelationships in radiata pine. For. Ecol. Manag. 2006, 229, 388–394, doi:10.1016/j.foreco.2006.04.019.
- Grabianowski, M.; Manley, B.; Walker, J.C.F. Acoustic measurements on standing trees, logs and green lumber. Wood Sci. Technol. 2006, 40, 205–216, doi:10.1007/s00226-005-0038-5.
- Achim, A.; Paradis, N.; Carter, P.; Hernández, R.E. Using acoustic sensors to improve the efficiency of the forest value chain in Canada: A case study with laminated veneer lumber. Sensors 2011, 11, 5716–5728, doi:10.3390/s110605716.
- Auty, D.; Achim, A. The relationship between standing tree acoustic assessment and timber quality in Scots pine and the practical implications for assessing timber quality from naturally regenerated stands. Forestry 2008, 81, 475–487, doi:10.1093/forestry/cpn015.
- Kumar, S. Genetic parameter estimates for wood stiffness, strength, internal checking, and resin bleeding for radiata pine. Can. J. For. Res. 2004, 34, 2601–2610, doi:10.1139/x04-128.
- Eckard, J.T.; Isik, F.; Bullock, B.; Li, B.; Gumpertz, M. Selection efficiency for solid wood traits in Pinus taeda using time-of-flight acoustic and micro-drill resistance methods. For. Sci. 2010, 56, 233–241.
- Ivkovic, M.; Gapare, W.J.; Abarquez, A.; Ilic, J.; Powell, M.B.; Wu, H.X. Prediction of wood stiffness, strength, and shrinkage in juvenile wood of radiata pine. Wood Sci. Technol. 2009, 43, 237–257, doi:10.1007/s00226-008-0232-3.
- Apiolaza, L.A. Very early selection for solid wood quality: Screening for early winners. Ann. For. Sci. 2009, 66, 601–611, doi:10.1051/forest/2009047.
- El-Kassaby, Y.A.; Mansfield, S.; Isik, F.; Stoehr, M. In situ wood quality assessment in Douglas-fir. Tree Genet. Genome. 2011, 7, 553–561, doi:10.1007/s11295-010-0355-1.
- Wielinga, B.; Raymond, C.A.; James, R.; Matheson, A.C. Effect of green density values on Pinus radiata stiffness estimation using a stress-wave technique. NZ J. For. Sci. 2009, 39, 71–79.
- Kennedy, R.W. Coniferous wood quality in the future: Concerns and strategies. Wood Sci. Technol. 1995, 29, 321–338, doi:10.1007/BF00202581.
- Gardiner, B.; Leban, J.M.; Auty, D.; Simpson, H. Models for predicting wood density of British-grown Sitka spruce. Forestry 2011, 84, 119–132, doi:10.1093/forestry/cpq050.
- Auty, D.; Gardiner, B.A.; Achim, A.; Moore, J.R.; Cameron, A.D. Models for predicting microfibril angle variation in Scots pine. Ann. For. Sci. 2013, 70, 209–218, doi:10.1007/s13595-012-0248-6.
- Lenz, P.; MacKay, J.; Rainville, A.; Cloutier, A.; Beaulieu, J. The influence of cambial age on breeding for wood properties in Picea glauca. Tree Genet. Genome. 2011, 7, 641–653, doi:10.1007/s11295-011-0364-8.
- Li, X.; Huber, D.A.; Powell, G.L.; White, T.L.; Peter, G.F. Breeding for improved growth and juvenile corewood stiffness in slash pine. Can. J. For. Res. 2007, 37, 1886–1893, doi:10.1139/X07-043.
- Gao, S.; Wang, X.; Wang, L.; Allison, R.B. Effect of temperature on acoustic evaluation of standing trees and logs: Part 2: Field investigation. Wood Fib. Sci. 2013, 45, 15–25.
- Evans, R. Rapid measurement of the transverse dimensions of tracheids in radial wood sections from Pinus radiata. Holzforschung 1994, 48, 168–172, doi:10.1515/hfsg.19126.96.36.199.
- Evans, R. A variance approach to the X-ray diffractometric estimation of microfibril angle in wood. Appita J. 1999, 52, 283–289.
- Megraw, R.; Leaf, G.; Bremer, D. Longitudinal shrinkage and microfibril angle in loblolly pine. In Proceedings of IAWA/IUFRO International Workshop on Microfibril Angle in Wood, Westport, New Zealand, 11–13 November 1997; Butterfield, B, Ed.; University of Canterbury: Christchurch, New Zealand, 1998; pp. 27–61.
- Littell, R.C.; Milliken, G.A.; Stroup, W.W.; Wolfinger, R.D.; Schabenberger, O. SAS for Mixed Models, 2nd ed. ed.; SAS Publishing: Cary, NC, USA, 2006.
- Holland, J.B. Estimating genotypic correlations and their standard errors using multivariate restricted maximum likelihood estimation with SAS Proc MIXED. Crop Sci. 2006, 46, 642–654, doi:10.2135/cropsci2005.0191.
- Lynch, M.; Walsh, B. Genetics and Analysis of Quantitative Characters; Sinauer: Sunderland, MA, USA, 1998.
- Laird, N.M.; Ware, J.H. Random-effects models for longitudinal data. Biometrics 1982, 38, 963–974, doi:10.2307/2529876.
- Akaike, H. A new look at the statistical model identification. IEEE Trans. Automat. Control 1974, 19, 716–723, doi:10.1109/TAC.1974.1100705.
- Parresol, B.R. Assessing tree and stand biomass: A review with examples and critical comparisons. For. Sci. 1999, 45, 573–593.
- Kumar, S.; Jayawickrama, K.J.S.; Lee, J.; Lausberg, M. Direct and indirect measures of stiffness and strength show high heritability in a wind-pollinated radiata pine progeny test in New Zealand. Silvae Genet. 2002, 51, 256–261.
- Timell, T. Compression Wood in Gymnosperms; Springer Verlag: Berlin, Germany, 1986.
- Zobel, B.J.; Van Buijtenen, J.P. Wood Variation: Its Causes and Control; Springer-Verlag: Heidelberg, NY, USA, 1989.
- Park, Y.S.; Weng, Y.; Mansfield, S.D. Genetic effects on wood quality traits of plantation-grown white spruce (Picea glauca) and their relationships with growth. Tree Genet. Genome 2012, 8, 303–311, doi:10.1007/s11295-011-0441-z.
- Liu, C.; Zhang, S.Y.; Cloutier, A.; Rycabel, T. Modeling lumber bending stiffness and strength in natural black spruce stands using stand and tree characteristics. For. Ecol. Manag. 2007, 242, 648–655, doi:10.1016/j.foreco.2007.01.077.
- Paradis, N.; Auty, D.; Carter, P.; Achim, A. Using a standing-tree acoustic tool to identify forest stands for the production of mechanically-graded lumber. Sensors 2013, 13, 3394–3408, doi:10.3390/s130303394.
- Lindström, H.; Harris, P.; Sorensson, C.T.; Evans, R. Stiffness and wood variation of 3-year old Pinus radiata clones. Wood Sci. Technol. 2004, 38, 579–597, doi:10.1007/s00226-004-0249-1.
- Zhang, H.; Wang, X.; Su, J. Experimental investigation of stress wave propagation in standing trees. Holzforschung 2011, 65, 743–748.
- Apiolaza, L.A.; Chauhan, S.S.; Walker, J.C.F. Genetic control of very early compression and opposite wood in Pinus radiata and its implications for selection. Tree Genet. Genome 2011, 7, 563–571, doi:10.1007/s11295-010-0356-0.
- Perron, M.; DeBlois, J.; Desponts, M. Use of resampling to assess optimal subgroup composition for estimating genetic parameters from progeny trials. Tree Genet. Genome 2012, 9, 129–143, doi:10.1007/s11295-012-0540-5.
© 2013 by the authors; licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution license (http://creativecommons.org/licenses/by/3.0/).